Atomic layer deposition of crystalline molybdenum oxide thin
and phase control by post-deposition annealing
, Peter J. Kinga
, Leonid Khriachtcheva,1
, Mikko J. Heikkil
, Simon Rushworthb
, Kenichiro Mizohatac
, Kristoffer Meinanderc
, Mikko Ritalaa
, Markku Leskel
aa aDepartment of Chemistry, University of Helsinki, P.O. Box 55, FI-00014, Finland bEpiValence Ltd, The Wilton Centre, Redcar, Cleveland, TS10 4RF, UK
cDivision of Materials Physics, Department of Physics, University of Helsinki, P.O. Box 43, FI-00014, Finland
a r t i c l e i n f o
Received 9 March 2018 Received in revised form 11 April 2018
Accepted 30 April 2018 Available online 11 May 2018
Atomic layer deposition Molybdenum oxide MoO3
a b s t r a c t
Molybdenum forms a range of oxides with different stoichiometries and crystal structures, which lead to different properties and performance in diverse applications. Herein, crystalline molybdenum oxide thin ﬁlms with controlled phase composition are deposited by atomic layer deposition. The MoO2(thd)2and O3as precursors enable well-controlled growth of uniform and conformalﬁlms at 200e275C. The as-depositedﬁlms are rough and, in most cases, consist of a mixture ofa- andb-MoO3as well as an un-identiﬁed suboxide MoOx(2.75x2.89) phase. The phase composition can be tuned by changing deposition conditions. Theﬁlm stoichiometry is close to MoO3and theﬁlms are relatively pure, the main impurity being hydrogen (2e7 at-%), with1 at-% of carbon and nitrogen. Post-deposition annealing is studiedin situby high-temperature X-ray diffraction in air, O2, N2, and forming gas (10% H2/90% N2) atmospheres. Phase-pureﬁlms of MoO2anda-MoO3are obtained by annealing at 450C in forming gas and O2, respectively. The ability to tailor the phase composition of MoOxﬁlms deposited by scalable atomic layer deposition method represents an important step towards various applications of molyb-denum oxides.
©2018 The Authors. Published by Elsevier Ltd. This is an open access article under the CC BY license (http://creativecommons.org/licenses/by/4.0/).
Molybdenum oxides (MoOx) form a versatile group of materials as their properties vary widely as a function of the molybdenum oxidation state. The most common molybdenum oxides are the monoclinic dioxide (MoO2) and the trioxide (MoO3), the latter of which exists in stable orthorhombic
aand metastable monoclinic
bphases. In addition, many crystalline mixed-valence suboxides with compositions between MoO2.75and MoO3are known, including the
hphases of Mo4O11(x¼2.75), Mo17O47(xz2.76), Mo5O14 (x¼2.80), and Mo8O23(xz2.88) as well as Mo9O26(xz2.89) in the monoclinic and triclinic (“Mo18O52”) phases[2e4]. The versa-tility of molybdenum oxides is reﬂected in, for example, the elec-trical properties at room temperature:
b-MoO3are relatively insulating with band gaps of approximately 3 eV(resistivity
Ucm)[5e7], Mo9O26 is a semiconductor (
Ucm)[8,9]and the well-known MoO2(
Ucm)are highly conducting. Addi-tionally, oxygen vacancies or reactions with hydrogen occur easily for MoO3, leading to oxygen deﬁcient, n-type semiconductor MoO 3-yor hydrogen bronzes HzMoO3.Partial reduction of molybdenum is accompanied by an increase in electrical conductivity [4,11e14]. Amorphous MoOx is also common with varying stoichiometries and, consequently, with different properties[15e17].
Due to the possible changes in the structure and oxidation state of molybdenum, molybdenum oxides show changes in optical properties upon excitation by light, heat, or applied voltage, i.e., photochromism [13,15,16,18], thermochromism [18,19], and elec-trochromism, respectively. The most widely studied applica-tions of the chromatic phenomena lie in smart windows and other optical coatings, but chromatic metal oxides may also be useful for displays and optical memories, for example[21,22]. Other ap-plications for MoO3and MoO3-yinclude catalysis[23,24], gas sen-sors , resistive switching memories , and lithium ion
E-mail address:miika.mattinen@helsinki.ﬁ(M. Mattinen). 1 Dedicated in memory of Dr. Leonid Khriachtchev.
Contents lists available atScienceDirect
Materials Today Chemistry
j o u r n a l h o m e p a g e :w w w . j o u r n a l s . e l s e v i e r . c o m / m a t e r i a l s - t o d a y - c h e m i s t r y /
batteries . Notably,
a-MoO3 has a two-dimensional crystal structure and a larger band gap than the most known 2D materials, such as transition metal dichalcogenides akin to MoS2. The 2D
a-MoO3 has shown promise as a channel , contact , and electron acceptor  material in ﬁeld-effect transistors. In gas sensors the 2D
a-MoO3has shown enhanced performance over its bulk counterpart. Many of the applications of MoO2are similar to those of MoO3and MoO3-y, including catalysisor lithium ion batteries . Reported applications of the crystalline suboxides with 2.75x2.89 are quite sparse, but some investigations have been made regarding lithium ion batteries[33e35]and catalysis [36,37].
Different MoOxphases show varying performance in different applications. For example, the layered structure of
a-MoO3allows it to outperform
b-MoO3in gasochromic applications, whereas
b-MoO3has been suggested to be more active for catalytic oxida-tion of methanol . Oxygen-deﬁcient MoO3-y has also been proposed to exhibit higher activity than MoO3in some photo- and electrocatalytic applications[1,40]. It has also been suggested that the crystalline suboxides may, at least in some cases, be the actual active species in catalysts considered to be MoO3. In addition to the phase, ﬁlm morphology is often crucial; in particular, high roughness or porosity of MoOxhas been found beneﬁcial for elec-trocatalysis, gas sensors, and lithium ion batteries, among other applications[40e43].
For many of the abovementioned applications, either uniform thinﬁlms or nanoparticles with controlled sizes and morphologies are required. Atomic layer deposition (ALD) is an advanced gas phase thinﬁlm deposition method, which relies on alternating self-limiting surface reactions. Therefore, ALD is able to coat large areas as well as substrates with complex shapes with a thickness uni-formity unmatched by any other method. ALD also typically de-posits high-qualityﬁlms at relatively low deposition temperatures. In addition, due to the cyclic nature of ALD, ﬁlm thickness and doping can be controlled accurately[44e46].
Reports on ALD of metal oxides have been very common since the 1990s, but theﬁrst report on the ALD of molybdenum oxide was published as late as in 2011 by Diskus et al., who used Mo(CO)6 with“wet ozone”, i.e. simultaneous exposure to O3and H2O, as the reactant. Since 2014, a range of new MoOxprocesses have been pub-lished, including Mo(CO)6 with O2plasma, Mo(NtBu)2(NMe2)2 with either O3or O2plasma[50,51], MoO2(tBuAMD)2with O3, MoO2(iPrAMD)2with O3, Mo(CpSiMe3)(CO)2(2-methylallyl) with O3as well as the only H2O-based process, Mo(ethylbenzene)2 with H2O. The composition of the depositedﬁlms, if reported, has usually been close to MoO3 [47,49e51,53,54,56], except for the Mo(VI)oxynitrideﬁlms deposited from MoO2(tBuAMD)2and O3 .
Deposition of crystalline (
a-MoO3)ﬁlms by ALD has only been reported from Mo(NtBu)2(NMe2)2 and O2 plasma at 250 C and above . Diskus et al.managed to crystallize the initially amorphous MoOx ﬁlms deposited from Mo(CO)6 and wet O3 to either
a-MoO3or a mixture of
b-MoO3depending on the annealing temperature. Nevertheless, the aforementioned ap-proaches to produce crystalline ﬁlms rely on either the use of plasma, which is problematic regarding conformality as well as batch processing, or post-deposition annealing, which is not suit-able for temperature-sensitive substrates. Furthermore, to the best of our knowledge, neither MoO2nor any of the crystalline suboxide phases (2.75 x 2.89) have been achieved by ALD, with or without post-deposition annealing. More generally, reports on thin ﬁlms of the suboxides are also scarce, which hinders their application.
We report theﬁrst ALD process capable of depositing crystalline molybdenum oxideﬁlms without the use of plasma, using a new
ALD precursor MoO2(thd)2 with O3 as the reactant. The growth characteristics were studied, followed by detailedﬁlm character-ization. Post-deposition annealing experiments were performed usingin situhigh-temperature X-ray diffraction in both reducing and oxidizing atmospheres. Annealing was then optimized to produce phase-pureﬁlms of
2.1. Film deposition
Molybdenum oxide thin ﬁlms were deposited using a com-mercial, hot wallﬂow-type F120 ALD reactor. Nitrogen (N2, AGA, 99.999%) was used as both carrier and purge gas at aﬂow rate of 400 sccm. The reactor pressure was on the order of 5 mbar. The deposition temperature varied by no more than±2C during each deposition, mostly towards higher temperatures due to overshoot during heating of the reactor. The ﬁlms were deposited on 55 cm2silicon (100) and soda lime glass substrates. The glass substrates were cleaned in an ultrasonic bath using successive baths of an alkaline ultrasonic cleaning solution, ethanol, and de-ionized water. The silicon wafers were used as-received.
Dioxobis(2,2,6,6-tetramethylheptane-3,5-dionato)molybde-num(VI) (MoO2(thd)2, 99.5%, EpiValence) was evaporated from an open glass boat heated to 135C inside the ALD reactor, slightly above the melting point of the precursor, which was about 130C under the ALD reactor conditions. A Mettler Toledo STARe system equipped with a TGA850 thermobalance was used for simultaneous thermogravimetric analysis (TGA) and differential thermal analysis (DTA) of the precursor. The TGA/DTA measurement was performed at atmospheric pressure ofﬂowing N2using a heating rate of 10C/ min and a sample size of approximately 10 mg.
Ozone (O3) was produced from oxygen (O2, AGA, 99.999%) using an ozone generator (Wedeco Ozomatic Modular 4 HC). The nominal O3concentration was 100 g/Nm3and theﬂow rate of the O3eO2 mixture was typically set to approximately 200 sccm using a needle valve. Unless otherwise noted,ﬁlms were deposited at 250C using 1 s MoO2(thd)2and 3 s O3pulses separated by 1 s N2purges.
2.2. Thickness measurements
Film thicknesses were measured by ellipsometry using a Film Sense FS-1 Multi-Wavelength instrument. The model used toﬁt the data consisted of four layers (silicon, native silicon oxide, dense MoOxbottom layer, and rough MoOxtop layer). The rough top layer was necessary to obtain good agreement between the data and the model and it was implemented using an effective medium approximation with 50% of the layer being void and the other 50% having properties of the dense MoOx layer underneath. Cauchy model was used for layers other than the silicon substrate. For comparison, UVeVIS spectroscopy (Hitachi U2000) and energy-dispersive X-ray spectrometry (EDS, Oxford INCA 350 connected to Hitachi S-4800) were also used for some samples to conﬁrm the thicknesses measured by ellipsometry. The high roughness of most ﬁlms prevented the use of X-ray reﬂectivity (XRR).
2.3. Film characterization
Film crystallinity was examined by X-ray diffraction (XRD) using a PANalytical X'Pert Pro MPD instrument in grazing incidence (incident angle of 1) geometry and a Cu K
l¼1.54 Å) X-ray beam. Composition of the surface layers was analyzed by X-ray photoelectron spectroscopy (XPS) using an Argus spectrometer (Omicron NanoTechnology GmbH). The samples were illuminated with X-rays emitted from a standard Mg source (K
aline) at a photon energy of 1253.6 eV. Binding energies were calibrated using the C 1s peak (284.8 eV) of ambient hydrocarbons, and peakﬁtting was done using the CasaXPS software. Film composition was analyzed by time-of-ﬂight elastic recoil detection analysis (ToF-ERDA) using a 40 MeV127I7þion beam.
Micro-Raman spectra were measured in backscattering geom-etry using confocal Raman microscopes with 100 objectives. Measurements with a 325 nm laser were performed with a Horiba Jobin Yvon LabRam HR 800 instrument, whereas an NT-MDT Ntegra instrument was used with 532 nm and 633 nm lasers. Laser power was adjusted to a level where no deterioration of the sample occurred.
Optical transmission measurements of theﬁlms deposited on soda lime glass substrates were conducted using a Hitachi U-2000 UVeVis spectrophotometer.
2.4. High-temperature X-ray diffraction
In situ high-temperature XRD (HTXRD) measurements were performed using an Anton-Paar HTK1200N oven connected to a PANalytical X'Pert Pro MPD diffractometer with a Cu K
l¼1.54 Å) X-ray source. The measurements were done under atmospheric pressure of air, O2(AGA, 99.9999%), N2(AGA, 99.999%, further pu-riﬁed with an Entegris Gatekeeper puriﬁer), or forming gas (10% H2 in N2, AGA). During the experiments, the temperature was increased from 26 up to 666C with the temperature stabilized every 40 C for recording of a grazing incidence diffractogram (incident angle of 1). Recording each diffractogram took approxi-mately 35 min, and the heating between the measurements was done with a rate of 10C/min followed by a two minute stabiliza-tion period, which resulted in a total durastabiliza-tion of approximately 11 h for each HTXRD experiment.
The Anton-Paar oven was also used to produce annealedﬁlms for further analysis. Based on the HTXRD measurements, a tem-perature of 450C and an annealing time of 1 h (O2) or 3 h (forming gas) were selected. The heating rate was 10 C/min, whereas cooling to room temperature took approximately 30 min. Isothermal measurements with consecutively measured grazing incidence diffractograms were also done under similar conditions to follow the transformation processes in more detail.
3. Results and discussion
3.1. Film growth
Molybdenum oxide thinﬁlms were deposited by atomic layer deposition (ALD) using dioxobis(2,2,6,6-tetramethylheptane-3,5-dionato)molybdenum(VI) [MoO2(thd)2] and O3 as precursors. No appreciableﬁlm growth occurred using H2O or H2S as the reactant. The lack of reactivity with water is common for precursors con-taining
b-diketonate ligands. In contrast, some of them, including Mo(thd)3, have been found to react with H2S. To the best of our knowledge, MoO2(thd)2is a new ALD precursor, whereas it has been used for CVD of MoOxwith O2as a reactant at relatively high temperatures (350e430C).
Thermogravimetric analysis (TGA) showed that MoO2(thd)2 volatilized cleanly leaving a residue of less than 2% (Fig. 1). While a solid at room temperature, MoO2(thd)2 melted at approximately
130C, which is just below the source temperature used in this work and in agreement with literature values of 129e135 C [61,62], as indicated by DTA (Fig. 1) and visual observations during heating of the ALD reactor. The favorable thermal properties together with the commercial availability and reactivity with O3 make MoO2(thd)2an attractive ALD precursor.
Mostﬁlm growth experiments were done at 250C, the tem-perature which yielded the most uniform ﬁlms and the highest growth rates close to 1 Å/cycle. Due to the roughness of theﬁlms, measuringﬁlm thicknesses turned out to be rather challenging by ellipsometry and UVeVIS spectrometry, and impossible by XRR. However, a goodﬁt of the ellipsometry data was obtained by using a four-layer model consisting of a Si substrate, a native SiOxlayer, a dense MoOxlayer, and a rough MoOxsurface layer (Fig. 2a). Similar thickness values were also measured by UVeVIS spectrometry and EDS (Fig. S1, Supplementary data). The similar trends of the optical thicknesses (ellipsometry, UVeVIS) and the mass thicknesses (EDS) support the use of the ellipsometry-derived totalﬁlm thicknesses, including both the dense bottom layer and the rough top layer, in the following discussion.
A rather high growth rate of approximately 1.0 Å/cycle was reached with a MoO2(thd)2pulse of only 0.2 s (Fig. 2b). However, increasing the pulse length above 1.0 s led to a slight increase in the growth rate, which is likely due to precursor decomposition. Nevertheless, pulsing MoO2(thd)2alone for 1000 pulses of 1 s each resulted in noﬁlm growth to the accuracy of the thickness mea-surements. Thus, the precursor decomposition seems to occur mostly on the surface of the growing MoOx ﬁlm as opposed to decomposition in the gas phase. From the average slope of the growth rate versus MoO2(thd)2pulse length from 0.2 to 3.0 s the decomposition was estimated to increase the growth rate by approximately 0.1 Å/cycle per second of MoO2(thd)2 pulsing. Therefore, the decomposition contributed only 2% of the growth rate when using 0.2 s pulses, which already appeared to be long enough to saturate the ALD-like surface reactions. Furthermore, the depositedﬁlms were uniform over the 55 cm2substrates with non-uniformities below 5%. With ozone, a 2 s pulse was needed to reached saturated growth rate (Fig. 2c).
Interesting effects were observed when theﬁlm thickness was varied: during theﬁrst 100 cycles theﬁlm growth was linear but slow with a growth rate of 0.35 Å/cycle and no apparent nucleation delay (Fig. 2d). The growth was also linear between 250 and 1000 cycles, but with a much higher growth rate of 1.25 Å/cycle. Furthermore, the thinnestﬁlms could be modeled as a single, dense
layer, whereas the thickerﬁlms required a rough surface layer in the model. The dramatic increase in roughness and growth rate between 100 and 250 cycles is linked to crystallization of theﬁlms, as will be discussed in Section3.2. Indeed, Vos et al.noted a similar effect with their ALD MoOx ﬁlms grown from Mo(N-tBu)2(NMe2)2and O2plasma at 300C, although they measured a
growth rate increase of only 25% upon crystallization compared to the 250% increase measured here. The difference may at least partly be explained by the high roughness of our ﬁlms as well as the different chemical reactions in thermal versus plasma-enhanced ALD. Large, 1.4e4-fold increases in growth rates upon crystalliza-tion have also been observed with ALD TiO2ﬁlms, which has been suggested to be due to both increased roughness and differences in surface chemistry, such as hydroxyl group coverage[63e65].
Varying the purge times from 1 to 5 s after each precursor pulse had no effect on the growth rate (Fig. 2e), as is expected for ALD. Pulse times of 1 s for MoO2(thd)2, 3 s for O3, and purges of 1 s were selected for further experiments.
The ﬁlm growth was rather sensitive to the deposition tem-perature, with the highest growth rates of approximately 1.0e1.1 Å/ cycle observed between 245 and 255C (Fig. 2f). The growth rate decreased strongly on both sides of this temperature range, which is attributed to slower crystallization at temperatures below 245C and, possibly, changes in the crystalline phase composition forﬁlms deposited at temperatures above 255C. The latter would require different phases to have different growth rates, perhaps due to differing catalytic activity or hydroxyl group coverage. Additionally, the surface area of theﬁlms may change with deposition temper-ature, which would affect the growth rate. Theﬁlms deposited at 300C showed increased non-uniformity, whereasﬁlms deposited at other temperatures were visibly uniform over the 5 5 cm2 substrates used in this work. Furthermore, despite the slight
precursor decomposition at 250C, highly conformal ﬁlms were deposited on trenches with a high aspect ratio of 30:1 within the uncertainty of the thickness measurements of approximately ±5 nm (Fig. 3).
Fig. 2.(a) Illustration of the ellipsometry model used in this work. Growth rates versus (b) MoO2(thd)2and (c) O3pulse lengths. (d) Film thickness versus the number of ALD cycles (inset shows 0e100 cycles). Growth rates extracted from linearﬁts to the data are indicated. Growth rates versus (e) purge lengths (only total thickness is shown for clarity) and (f) deposition temperature. Unless otherwise noted, 1000 cycles with 1 s MoO2(thd)2and 3 s O3pulses and 1 s purges were applied at 250C.
The ﬁlm crystallinity was ﬁrst examined by XRD. For an approximately 100 nm ﬁlm deposited at 250 C, multiple re-ﬂections originating from both the stable orthorhombic
aand metastable monoclinic
bphases of MoO3 were detected by grazing incidence XRD (Fig. 4a). In addition, a strong reﬂection was detected at approximately 22.4 2
qaccompanied by a second reﬂection close to 462
q, which corresponds to half the d-spacing of theﬁrst peak. These peaks could not be indexed to either of the MoO3phases. Instead, several known suboxide phases, including
h-Mo4O11, Mo17O47 , Mo5O14, Mo8O23 , Mo9O26, and Mo18O52have reﬂections close to these positions. The three partially overlapping peaks at 22.4 (suboxide), 23.0 [
b-MoO3 (011)] and 23.32
a-MoO3(110)] were the most intense for each phase also in the
qgeometry (Fig. S2, Supplementary data) and the relative peak intensities were also rather similar to the GIXRD measurements. Thus, taking into ac-count the well-known differences between GIXRD and
qge-ometries and the planes detected by them, none of the phases appears to be strongly textured.
Raman spectroscopy was also used to study the phase compo-sition.
bphases of MoO3were detected with UV (325 nm), green (532 nm), and red (633 nm) lasers, although the
relative intensities of the peaks were different for each laser (Fig. 4b). However, no signs of any suboxide phase were seen with any of the lasers. Both
h-Mo4O11have been reported to be relatively weakly Raman active when excited with a green (514.5 or 532 nm) laser[78,79], but increased Raman activity under red (633 nm) laser illumination has been noted for these phases [78,80]. Mo18O52 has been reported to be weakly Raman active under IR (1064 nm), red (633 nm), and UV (244 nm) lasers, whereas relatively strong peaks should result from Mo8O23 when using either a 633 or 244 nm laser. To the best of our knowledge, Raman spectra of other suboxide phases, such as Mo17O47, Mo5O14, or Mo9O26, have not been reported.
Deposition temperature had a strong effect onﬁlm morphology (Fig. 5) as well as crystallinity (Fig. 6). Theﬁlm deposited at 200C appeared smooth and nearly featureless, in line with its amorphous structure. At 225C rod-like crystallites of an unidentiﬁed suboxide phase formed. Theﬁlms deposited between 240 and 255C had rather similar morphologies with rough surfaces composing of both rod and plate-like crystallites, and theﬁlms contained both the
bphases of MoO3 in addition to the suboxide phase(s). At 260C plate-like crystallites started to dominate the surface, which was accompanied by a strong decrease in the XRD reﬂection orig-inating from the suboxide (2
qz22.4), while both MoO3phases were still present. The dominantly plate-like ﬁlms deposited at 275e300C were nearly phase-pure
a-MoO3with slight traces of
b-MoO3. In addition, the changes in the relative intensities of the
a-MoO3peaks at temperatures above 260C suggest changes in their orientation.
We also observed that precursor pulse times had some effect on the ﬁlm morphology and phase composition: long MoO2(thd)2 pulses led to more plate-like morphology with increased amount of
a-MoO3 compared to the suboxide and
b-MoO3 (Fig. S3, Supplementary data), whereas long O3 pulses decreased the amount of the suboxide with a corresponding increase in both the
b-MoO3phases (Fig. S4, Supplementary data). Even purge times affected ﬁlm morphology (Fig. S5, Supplementary data). There are at least two ways the pulse times may affect theﬁlm morphology and crystallinity at doses higher than those needed for saturation of the growth rate. First, longer pulses or purges give more time for processes such as crystallization, phase trans-formation, and surface diffusion. Second, increasing the dose of especially the reactant, such as ozone, may reduce the impurities, improve the stoichiometry, and affect theﬁlm structure.
Notable changes in the ﬁlm morphology (Fig. 7a andFig. S6, Supplementary data) as well as crystallinity (Fig. 7b) occurred at 250C with increasingﬁlm thickness. The thinnestﬁlms up to 100 cycles were smooth and amorphous, whereas a crystalline sub-oxide phase was formed after 250 cycles, which was accompanied by a strong increase in roughness. Thereafter the roughness continued to increase up to 1000 cycles, and changes in phase composition were also observed: both
b-MoO3formed after 500 cycles and their amounts relative to the suboxide seemed to increase with increasingﬁlm thickness. The observation of onset of crystallization between 100 and 250 cycles agrees well with the strong increase in the growth rate discussed in Section 3.1. The roughness of theﬁlms increases their surface area, which has been found beneﬁcial in many applications of MoOx, as discussed in the Introduction. Based on AFM images, the surface area of the roughest, 1000 cycleﬁlm was estimated to be approximately twice the substrate area.
Theﬁlms deposited at 225, 250, and 275C were all relatively pure. The main impurity was hydrogen, and some carbon and ni-trogen were also detected (Table 1). The O/Mo ratios were rather close to 3; this probably results from a balance of the suboxide MoOxphase (2.75x2.89) decreasing the ratio and the presence
of residual OHgroups increasing it. The highest hydrogen content was measured for theﬁlm deposited at 250C, which also had the highest O/Mo ratio, suggesting the incorporation of hydrogen as hydroxyl groups. The amount of carbon, which likely originates from the precursor, was low and decreased with increasing
deposition temperature. Interestingly, the ﬁlms contained small amounts of N (0.5e1 at-%). We think this has to be incorporated during the deposition from the usually inert N2carrier gas, as no nitrogen-containing chemicals were used in the precursor syn-thesis and the nitrogen appears to be distributed throughout the ﬁlm thickness. Molybdenum oxides have been reported to incor-porate nitrogen relatively easily. For example,ﬁlms deposited from a nitrogen-containing precursor MoO2(tBuAMD)2and O3by ALD were described as Mo(VI)oxynitride , partial nitridation of MoOxhas been reported upon N2annealing at 400C, and nitrogen impurities have also been found for MoOxﬁlms deposited under nominally nitrogen-free conditions.
X-ray photoelectron spectroscopy (XPS) showed that molybde-num on theﬁlm surface was mostly present as Mo6þ, as evidenced by the Mo 3d5/2 and Mo 3d3/2 binding energies of 233.0 and 236.2 eV, respectively (Fig. 8a). Approximately 10% of molybdenum was identiﬁed as Mo5þrepresented by a doublet with binding en-ergies of 231.3 (Mo 3d5/2) and 234.5 eV (Mo 3d3/2). The observed binding energies are within the range reported for different MoO3 samples, in particular close to the values for crystalline ALD
a-MoO3ﬁlms deposited by Vos et al.and somewhat higher than those reported for amorphous ALD MoO3 [49,53,56]. The Mo5þ content would be expected to range from 50% (Mo4O11) to 22% (Mo9O26) for the different suboxide phases. However, the similar Mo5þ/Mo6þratios for theﬁlms deposited at different temperatures point to changes on theﬁlm surface due to ambient exposure, as XRD showed theﬁlms deposited at 225 and 275C to be nearly phase-pure suboxide and
The majority of oxygen (Fig. 8b) was present as oxide ions (O2), whereas about 5% (275C) or 12% (225 and 250C) of oxygen was identiﬁed as hydroxyl groups (OH). The O 1s binding energies of 530.7 (O2) and 531.9 eV (OH) are in relatively good agreement with other ALD MoO3ﬁlms[49,51,56]. A minor O 1s component at 533.3 eV was attributed to organic species containing oxygen, in accordance with detection of carbonyl species in C 1s spectra (not shown).
Optical properties were evaluated from theﬁlms deposited on soda lime glass substrates. Using a Tauc plot, an indirect band gap of 2.8 eV was extracted for a 2000 cycle ﬁlm deposited at 250 C (Fig. S7, Supplementary data), which is within the range of band gap values (2.7e3.2 eV) reported for MoO3[1,7,51,83]. The refractive indices at 580 nm ranged from 2.0 for the amorphousﬁlms to 2.2 for the predominantly
a-MoO3ﬁlms deposited at 275e300C and
Fig. 5.SEM images of MoOxﬁlms deposited on silicon at different temperatures using 1000 cycles.
even 2.4e2.5 for the mixed-phase ﬁlms deposited at 250 C. Refractive indices ranging from 1.8 to 2.2 have been reported for trioxide-like MoOx ﬁlms [7,51,83]. Thus, the highest values measured for the mixed-phaseﬁlms may be due to the suboxide phase(s).
3.3. Post-deposition annealing
The phase composition of the MoOx ﬁlms could be tuned by changing the deposition conditions. However, the majority of the depositedﬁlms were mixtures of three phases. Additional control in phase composition was sought through post-deposition
annealing. Approximately 100 nm thick MoOx ﬁlms deposited at 250C (1000 cycles), which consisted of a mixture of suboxide,
b-MoO3 phases, were selected for annealing experi-ments performed in both oxidizing and reducing atmospheres. The effects of annealing were followedin situby HTXRD.
Upon annealing in O2theﬁrst changes occurred above 306 and 346 C, when the suboxide and metastable
b-MoO3 phases, respectively, disappeared (Fig. 9). From 386 to 586C theﬁlm was phase-pure
a-MoO3, the only changes being peak shifts due to anisotropic thermal expansion and variation in relative peak in-tensities (preferred orientation). Above 586 C, the
a-MoO3ﬁlm sublimed, leaving a bare silicon substrate, as veriﬁed by EDS. The
Fig. 7.(a) SEM images and roughness values (Rq) measured by AFM and (b) grazing incidence X-ray diffractograms of MoOxﬁlms of different thicknesses deposited on silicon at 250C.aandbrefer toa-MoO3andb-MoO3, whereas suboxide denotes an unidentiﬁed MoOx(2.75x2.89) phase.
Elemental compositions analyzed by ToF-ERDA for MoOxﬁlms deposited at different temperatures on silicon using 1000 cycles.
Deposition temperature (C) Mo (at-%) O (at-%) O/Mo C (at-%) H (at-%) N (at-%)
225 24.0±1.2 71.2±2.9 2.97±0.19 1.3±0.5 3.0±1.2 0.58±0.24
250 22.0±0.5 70.1±1.3 3.19±0.10 0.47±0.15 6.6±1.1 0.92±0.15
275 24.4±1.0 73.2±2.4 3.01±0.16 0.11±0.07 1.8±0.8 0.56±0.22
onset temperature for the sublimation of
a-MoO3 has been re-ported to be 500e700C depending on experimental conditions [84,85]. Attempts to produce ultrathin, 2D
a-MoO3 ﬁlms from amorphous, sub-5 nm MoOxﬁlms were unsuccessful, as no crys-tallization was detected by either in situ or ex situ XRD after annealing in O2to 450C or higher temperatures.
Forming gas (10% H2/90% N2) provided a reducing atmosphere in order to produce MoO2ﬁlms. Theﬁrst changes in HTXRD mea-surements were observed above 226 C (Fig. 10), when
b-MoO3 disappeared and the initial suboxide phase transformed to a new phase, most likely monoclinic
h-Mo4O11. At 386C,
h-Mo4O11 may have converted to another suboxide phase and
a-MoO3had disappeared with MoO2 starting to form. The formation of
h-Mo4O11 is further supported by isothermal measurements pre-sented later in this section. Between 426 and 546C, theﬁlm was phase-pure, monoclinic MoO2 (tugarinovite) . Starting at 586 C, MoO2 disappeared and a few broad reﬂections appeared that most likely originate from molybdenum silicide(s).
An HTXRD experiment was also performed in air, which yielded results very similar to O2(not shown). Annealing in N2, on the other hand, produced a complex mixture of MoOx phases (Fig. S8, Supplementary data). Multiple peaks arising from suboxide pha-se(s) appeared at 386C.
b-MoO3 disappeared by 426C and
a-MoO3by 626C leaving only the suboxide phase(s) between 626 and 666C, where the heating was stopped.
Further insight into the production of phase-pure
a-MoO3and MoO2 ﬁlms in O2 and forming gas, respectively, was obtained through isothermal HTXRD measurements. The transformation to
a-MoO3was rapid in O2atmosphere at 450C; only
a-MoO3was detected after annealing for 35 min and no changes in peak in-tensities were seen when the annealing was continued (Fig. S9, Supplementary data). MoO2 formed more slowly in forming gas at 450C (Fig. S10, Supplementary data): after 35 min of annealing
b-MoO3 and the initial suboxide phase had disappeared, but
a-MoO3remained and an intermediate phase identiﬁed as
h-Mo4O11 had formed along with some traces of MoO2. The
h-Mo4O11 intermediate, which has been commonly observed when reducing MoO3to MoO2[87,88], was completely removed and formation of MoO2 ﬁnished after annealing for 140 min. Further annealing caused no changes in the diffractograms.
3.4. Characterization of annealedﬁlms
The MoO2ﬁlms formed by annealing in forming gas at 450C had a very rough morphology consisting ofﬂower-like structures with widths of about 1
mm (Fig. 11a). Between these structures a smoother area was exposed. The
a-MoO3ﬁlms formed by the O2 annealing at 450C consisted of plate-like crystallites on the sur-face with roughness comparable to the as-depositedﬁlm (Fig. 11b). Theﬁlm formed after the HTXRD measurement in forming gas ending at 666C was found to be a mixture of tetragonal
a-MoSi2 and Mo5Si3phases with an additional reﬂection that we were un-able to identify (Fig. S11a, Supplementary data). The morphology and roughness of thisﬁlm were rather similar to the as-deposited ﬁlm (Fig. S11b, Supplementary data). The formation of silicides is attributed to reactions between theﬁlm and the silicon substrate. It is plausible that MoO2isﬁrst reduced to metallic Mo, which has been reported to occur, although very slowly, at temperatures as low as 500C in 10% H2. MoSixis then formed upon reaction of Moﬁlm with the Si substrate, which has been reported to proceed at 500C and above. Therefore, it seems that metallic Moﬁlms could be obtained upon reduction in forming gas at approximately 600C if the Si substrate was covered by a suitable diffusion barrier layer.
a-MoO3ﬁlm produced by annealing in O2 showed lower levels of H and N compared to the as-depositedﬁlm, with slightly over stoichiometric O/Mo ratio of 3.15±0.11 (Table 2). The MoO2 ﬁlm resulting from annealing in forming gas had an O/Mo ratio of 2.11±0.05 and theﬁlm was the purest of all analyzedﬁlms with sub-at-% carbon, nitrogen, and hydrogen contents. Whereas ToF-ERDA provides results averaged through the wholeﬁlm thickness, the surface was speciﬁcally probed by XPS.
The as-deposited and oxygen-annealedﬁlms appeared to have nearly identical surface composition with some 90% of Mo present as Mo6þand 10% as Mo5þ(Fig. S12a, Supplementary data). The O 1s component at 531.9 eV attributed to hydroxyl groups, however, was approximately halved by the O2annealing (Fig. S12b). Mo4þwas expectedly detected after the forming gas annealing with Mo 3d5/2 and 3d3/2 binding energies of 229.7 and 232.9 eV, respectively, although the relative amounts of Mo4þ, Mo5þ, and Mo6þ were approximately identical on the surface. This is likely due to surface
Fig. 10.High-temperature grazing incidence X-ray diffractograms (left) of a MoOxﬁlm heated in forming gas (10% H2/90% N2) from 26 to 666C, where white and black represent low and high intensities, respectively. On right, peaks between 20 and 352qare identiﬁed at selected temperatures to highlight the phase transitions.aandbrefer toa-MoO3and b-MoO3, whereas suboxide denotes an unidentiﬁed MoOx(2.75x2.89) phase.
Fig. 11.Grazing incidence X-ray diffractograms (top row) and SEM images together with roughness values measured by AFM (bottom row) of (a) MoO2ﬁlm produced by annealing in forming gas (450C, 3 h) and (b)a-MoO3ﬁlm produced by annealing in O2(450C, 1 h).
Elemental compositions of annealed MoOxﬁlms analyzed by ToF-ERDA. Theﬁlms were deposited on silicon at 250C using 1000 cycles.
Treatment Mo (at-%) O (at-%) O/Mo C (at-%) H (at-%) N (at-%)
oxidation of the MoO2ﬁlm, as has been previously observed. Interestingly, the relative intensity of the 531.9 eV O 1s peak attributed to the OH groups increased after the forming gas annealing, although the hydrogen content throughout the ﬁlm analyzed by ToF-ERDA was negligible. This suggests that the hy-droxyl groups may have been exclusively present on theﬁlm sur-face in the forming gas annealedﬁlm, perhaps due to exposure to ambient air.
Atomic layer deposition of crystalline molybdenum oxide thin ﬁlms was demonstrated using a new, commercially available pre-cursor MoO2(thd)2with O3. Well controlledﬁlm growth with good uniformity and conformality was achieved although complete saturation was not reached with MoO2(thd)2. Most of the ﬁlms were mixtures of
b-MoO3, and an unidentiﬁed suboxide MoOxphase (2.75x2.89). Theﬁlm composition was close to MoO3and the ﬁlms had fairly low levels of impurities. Relative amounts of the different phases could be controlled by changing the deposition conditions. Post-deposition annealing treatments studied by high-temperature X-ray diffraction enabled further control ofﬁlm composition. In particular, single-phase
a-MoO3and MoO2ﬁlms were achieved by annealing in O2 and forming gas, respectively. As the thickness, crystallinity, morphology, and phase composition strongly affect the performance of MoOx ﬁlms, the presented ALD process constitutes an important step towards the use of MoOxin various applications such as sensing, energy storage, and catalysis.
Declarations of interest
The research was supported by the Finnish Centre of Excellence in Atomic Layer Deposition funded by Academy of Finland and ASM Microchemistry. Ms. Kati Meril€ainen and Mr. Mikko Kaipio are acknowledged for their help with the Raman and HTXRD mea-surements, respectively. Mr. Niklas Stegmann is thanked for assis-tance in thickness measurements and Mr. Tomi Iivonen and Mr. Georgi Popov are acknowledged for helping with the UVeVIS measurements.
Appendix A. Supplementary data
Supplementary data related to this article can be found at https://doi.org/10.1016/j.mtchem.2018.04.005.
 I.A. de Castro, R.S. Datta, J.Z. Ou, A. Castellanos-Gomez, S. Sriram, T. Daeneke, K. Kalantar-zadeh, Molybdenum oxidesefrom fundamentals to functionality, Adv. Mater. 29 (2017) 1701619.
 L. Kihlborg, Studies on molybdenum oxides, Acta Chem. Scand. 13 (1959) 954e962.
 L. Kihlborg, The crystal chemistry of molybdenum oxides, in: R. Ward (Ed.), Advances in Chemistry: Nonstoichiometric Compounds, American Chemical Society, Washington, D.C., 1963, pp. 37e45.
 H. Vincent, M. Mareio, On structural aspects of molybdenum bronzes and molybdenum oxides in relation to their low-dimensional transport properties, in: C. Schlenker (Ed.), Low-dimensional Electronic Properties of Molybdenum Bronzes and Oxides, Kluwer Academic Publishers, Dordrecht, The Netherlands, 1989, pp. 49e86.
 P.F. Carcia, E.M. McCarron, Synthesis and properties of thinﬁlm polymorphs of molybdenum trioxide, Thin Solid Films 155 (1987) 53e63.
 I. Navas, R. Vinodkumar, K.J. Lethy, A.P. Detty, V. Ganesan, V. Sathe, V.P. Mahadevan Pillai, Growth and characterization of molybdenum oxide
nanorods by RF magnetron sputtering and subsequent annealing, J. Phys. D Appl. Phys. 42 (2009) 175305.
 N. Miyata, S. Akiyoshi, Preparation and electrochromic properties of rf-sputtered molybdenum oxideﬁlms, J. Appl. Phys. 58 (1985) 1651e1655.  R.L. Smith, G.S. Rohrer, Scanning probe microscopy of cleaved molybdates:a
-MoO3(010), Mo18O52(100), Mo8O23(010), and h-Mo4O11(100), J. Solid State
Chem. 124 (1996) 104e115.
 M.S. da Luz, A. de Campos, B.D. White, J.J. Neumeier, Electrical resistivity, high-resolution thermal expansion, and heat capacity measurements of the charge-density wave compound y-Mo4O11, Phys. Rev. B 79 (2009) 233106.
 D.B. Rogers, R.D. Shannon, A.W. Sleight, J.L. Gillson, Crystal chemistry of metal dioxides with rutile-related structures, Inorg. Chem. 8 (1969) 841e849.  S. Balendhran, J. Deng, J.Z. Ou, S. Walia, J. Scott, J. Tang, K.L. Wang, M.R. Field,
S. Russo, S. Zhuiykov, M.S. Strano, N. Medhekar, S. Sriram, M. Bhaskaran, K. Kalantar-zadeh, Enhanced charge carrier mobility in two-dimensional high dielectric molybdenum oxide, Adv. Mater. 25 (2013) 109e114.
 K. Inzani, M. Nematollahi, F. Vullum-Bruer, T. Grande, T.W. Reenaas, S.M. Selbach, Electronic properties of reduced molybdenum oxides, Phys. Chem. Chem. Phys. 19 (2017) 9232e9245.
 T. He, J. Yao, Photochromism of molybdenum oxide, J. Photochem. Photobiol. C Photochem. Rev. 4 (2003) 125e143.
 X.K. Hu, Y.T. Qian, Z.T. Song, J.R. Huang, R. Cao, J.Q. Xiao, Comparative study on MoO3and HxMoO3nanobelts: structure and electric transport, Chem. Mater.
20 (2008) 1527e1533.
 J. Scarminio, A. Lourenço, A. Gorenstein, Electrochromism and photochro-mism in amorphous molybdenum oxideﬁlms, Thin Solid Films 302 (1997) 66e70.
 M. Rouhani, J. Hobley, G.S. Subramanian, I.Y. Phang, Y.L. Foo, S. Gorelik, The inﬂuence of initial stoichiometry on the mechanism of photochromism of molybdenum oxide amorphousﬁlms, Sol. Energy Mater. Sol. Cells 126 (2014) 26e35.
 J.H. Ku, J.H. Ryu, S.H. Kim, O.H. Han, S.M. Oh, Reversible lithium storage with high mobility at structural defects in amorphous molybdenum dioxide elec-trode, Adv. Funct. Mater. 22 (2012) 3658e3664.
 S.K. Deb, J.A. Chopoorian, Optical properties and color-center formation in thinﬁlms of molybdenum trioxide, J. Appl. Phys. 37 (1966) 4818e4825.  M.A. Arvizu, M. Morales-Luna, M. Perez-Gonzalez, E. Campos-Gonzalez,
O. Zelaya-Angel, S.A. Tomas, Inﬂuence of thermal annealings in argon on the structural and thermochromic properties of MoO3thinﬁlms, Int. J.
Thermo-phys. 38 (2017) 51.
 S.S. Kanu, R. Binions, Thinﬁlms for solar control applications, Proc. R. Soc. A Math. Phys. Eng. Sci. 466 (2009) 19e44.
 Y. Ohko, T. Tatsuma, T. Fujii, K. Naoi, C. Niwa, Y. Kubota, A. Fujishima, Mul-ticolour photochromism of TiO2ﬁlms loaded with silver nanoparticles, Nat.
Mater. 2 (2003) 29e31.
 J.N. Yao, K. Hashimoto, A. Fujishima, Photochromism induced in an electro-lytically pretreated MoO3thinﬁlm by visible light, Nature 355 (1992) 624e626.
 M.M. Bettahar, G. Costentin, L. Savary, J.C. Lavalley, On the partial oxidation of propane and propylene on mixed metal oxide catalysts, Appl. Catal. A Gen. 145 (1996) 1e48.
 G. Mestl, T.K.K. Srinivasan, Raman spectroscopy of monolayer-type catalysts: supported molybdenum oxides, Catal. Rev. Sci. Eng. 40 (1998) 451e570.  S.S. Sunu, E. Prabhu, V. Jayaraman, K.I. Gnanasekar, T.K. Seshagiri,
T. Gnanasekaran, Electrical conductivity and gas sensing properties of MoO3,
Sens. Actuators B 101 (2004) 161e174.
 M. Arita, H. Kaji, T. Fujii, Y. Takahashi, Resistance switching properties of molybdenum oxideﬁlms, Thin Solid Films 520 (2012) 4762e4767.  N.A. Chernova, M. Roppolo, A.C. Dillon, M.S. Whittingham, Layered vanadium
and molybdenum oxides: batteries and electrochromics, J. Mater. Chem. 19 (2009) 2526e2552.
 K.C. Santosh, R.C. Longo, R. Addou, R.M. Wallace, K. Cho, Electronic properties of MoS2/MoOxinterfaces: implications in tunnelﬁeld effect transistors and
hole contacts, Sci. Rep. 6 (2016) 33562.
 A.J. Molina-Mendoza, J.L. Lado, J.O. Island, M.A. Ni~no, L. Aballe, M. Foerster, F.Y. Bruno, A. Lopez-Moreno, L. Vaquero-Garzon, H.S.J. van der Zant, G. Rubio- Bollinger, N. Agraït, E.M. Perez, J. Fernandez-Rossier, A. Castellanos-Gomez, Centimeter-scale synthesis of ultrathin layered MoO3 by van der waals
epitaxy, Chem. Mater. 28 (2016) 4042e4051.
 F. Ji, X. Ren, X. Zheng, Y. Liu, L. Pang, J. Jiang, S. Liu, 2D-MoO3nanosheets for
superior gas sensors, Nanoscale 8 (2016) 8696e8703.
 O.G. Marin Flores, S. Ha, Activity and stability studies of MoO2catalyst for the
partial oxidation of gasoline, Appl. Catal. A Gen. 352 (2009) 124e132.  Y. Shi, B. Guo, S.A. Corr, Q. Shi, Y.-S. Hu, K.R. Heier, L. Chen, R. Seshadri,
G.D. Stucky, Ordered mesoporous metallic MoO2 materials with highly
reversible lithium storage capacity, Nano Lett. 9 (2009) 4215e4220.  L. Zhou, N. Ding, J. Yang, L. Yang, Y. Zong, Z. Liu, A. Yu, Sulfur encapsulated in
Mo4O11-anchored ultralight graphene for high-energy lithium sulfur
batte-ries, ACS Sustain. Chem. Eng. 4 (2016) 3679e3687.
 E. Shembel, R. Apostolova, V. Nagirny, I. Kirsanova, P. Grebenkin, P. Lytvyn, Electrolytic molybdenum oxides in lithium batteries, J. Solid State Electro-chem. 9 (2005) 96e105.
 P.A. Christian, J.N. Carides, F.J. DiSalvo, J.V. Waszczak, Molybdenum oxide cath-odes in secondary lithium cells, J. Electrochem. Soc. 127 (1980) 2315e2319.  B. Delmon, Solid state reactions in catalysts: an approach to real active
in Surface Science and Catalysis, vol. 111, Elsevier B.V., Amsterdam, Netherlands, 1997, pp. 39e51.
 E.M. Gaigneaux, M.J. Genet, P. Ruiz, B. Delmon, Catalytic behavior of molyb-denum suboxides in the selective oxidation of isobutene to methacrolein, J. Phys. Chem. B 104 (2000) 5724e5737.
 D. Di Yao, J.Z. Ou, K. Latham, S. Zhuiykov, A.P. O'Mullane, K. Kalantar-zadeh, Electrodepositeda- andb-phase MoO3ﬁlms and investigation of their
gaso-chromic properties, Cryst. Growth Des. 12 (2012) 1865e1870.
 C.J. Machiels, W.H. Cheng, U. Chowdhry, W.E. Farneth, F. Hong, E.M. McCarron, A.W. Sleight, The effect of the structure of molybdenum oxides on the se-lective oxidation of methanol, Appl. Catal. 25 (1986) 249e256.
 Z. Luo, R. Miao, T.D. Huan, I.M. Mosa, A.S. Poyraz, W. Zhong, J.E. Cloud, D.A. Kriz, S. Thanneeru, J. He, Y. Zhang, R. Ramprasad, S.L. Suib, Mesoporous MoO3exmaterial as an efﬁcient electrocatalyst for hydrogen evolution
re-actions, Adv. Energy Mater. 6 (2016).
 V.S. Saji, C.W. Lee, Molybdenum, molybdenum oxides, and their electro-chemistry, ChemSusChem 5 (2012) 1146e1161.
 N. Illyaskutty, H. Kohler, T. Trautmann, M. Schwotzer, V.P. Mahadevan Pillai, Hydrogen and ethanol sensing properties of molybdenum oxide nanorods based thin ﬁlms: effect of electrode metallization and humid ambience, Sensors Actuators B Chem. 187 (2013) 611e621.
 W. Li, F. Cheng, Z. Tao, J. Chen, Vapor-transportation preparation and reversible lithium intercalation/deintercalation ofa-MoO3microrods, J. Phys.
Chem. B 110 (2006) 119e124.
 M. Ritala, J. Niinisto, Atomic layer deposition, in: A.C. Jones, M.L. Hitchman€ (Eds.), Chemical Vapour Deposition: Precursors, Processes and Applications, Royal Society of Chemistry, Cambridge, 2009, pp. 158e206.
 S.M. George, Atomic layer deposition: an overview, Chem. Rev. 110 (2010) 111e131.
 M. Ritala, M. Leskel€a, Atomic layer deposition, in: H.S. Nalwa (Ed.), Handbook of Thin Film Materials, Academic, San Diego, 2002, pp. 103e159.
 M. Diskus, O. Nilsen, H. Fjellvåg, Growth of thinﬁlms of molybdenum oxide by atomic layer deposition, J. Mater. Chem. 21 (2011) 705.
 G. Song, G.H. Ryu, S.J. Lee, S. Sim, C.W. Lee, T. Choi, H. Jung, Y. Kim, Z. Lee, J.-M. Myoung, C. Dussarrat, C. Lansalot-Matras, J. Park, H. Choi, H. Kim, Controllable synthesis of molybdenum tungsten disulﬁde alloy for vertically composition-controlled multilayer, Nat. Commun. 6 (2015) 7817.
 A. Bertuch, G. Sundaram, M. Saly, D. Moser, R. Kanjolia, Atomic layer depo-sition of molybdenum oxide using bis(tert-butylimido)bis(dimethylamido) molybdenum, J. Vac. Sci. Technol. A 32 (2014), 01A119.
 B. Macco, M.F.J. Vos, N.F.W. Thissen, A.A. Bol, W.M.M. Kessels, Low-tempera-ture atomic layer deposition of MoOxfor silicon heterojunction solar cells,
Phys. Status Solidi Rapid Res. Lett. 9 (2015) 393e396.
 M.F.J. Vos, B. Macco, N.F.W. Thissen, A.A. Bol, W.M.M. Kessels, Atomic layer deposition of molybdenum oxide from (NtBu)2(NMe2)2Mo and O2plasma,
J. Vac. Sci. Technol. A 34 (2016), 01A103.
 A.R. Mouat, A.U. Mane, J.W. Elam, M. Delferro, T.J. Marks, P.C. Stair, Volatile hexavalent oxo-amidinate complexes: molybdenum and tungsten precursors for atomic layer deposition, Chem. Mater. 28 (2016) 1907e1919.
 T. Jurca, A.W. Peters, A.R. Mouat, O.K. Farha, J.T. Hupp, T.L. Lohr, M. Delferro, T.J. Marks, Second-generation hexavalent molybdenum oxo-amidinate pre-cursors for atomic layer deposition, Dalton Trans. 46 (2017) 1172e1178.  C.E. Nanayakkara, A. Vega, G. Liu, C.L. Dezelah, R.K. Kanjolia, Y.J. Chabal, Role of
initial precursor chemisorption on incubation delay for molybdenum oxide atomic layer deposition, Chem. Mater. 28 (2016) 8591e8597.
 T.L. Drake, P.C. Stair, Vapor deposition of molybdenum oxide using bis(e-thylbenzene) molybdenum and water, J. Vac. Sci. Technol. A 34 (2016) 51403.  M. Diskus, O. Nilsen, H. Fjellvåg, S. Diplas, P. Beato, C. Harvey, E. van Schrojen-stein Lantman, B.M. Weckhuysen, Combination of characterization techniques for atomic layer deposition MoO3coatings: from the amorphous to the
ortho-rhombica-MoO3crystalline phase, J. Vac. Sci. Technol. A 30 (2012), 01A107.
 T. Suntola, Atomic layer epitaxy, Thin Solid Films 216 (1992) 84e89.  J. Jokinen, J. Keinonen, P. Tikkanen, A. Kuronen, T. Ahlgren, K. Nordlund,
Comparison of TOF-ERDA and nuclear resonance reaction techniques for range proﬁle measurements of keV energy implants, Nucl. Inst. Methods Phys. Res. B 119 (1996) 533e542.
 M. Mattinen, T. Hatanp€a€a, T. Sarnet, K. Mizohata, K. Meinander, P.J. King, L. Khriachtchev, J. R€ais€anen, M. Ritala, M. Leskel€a, Atomic layer deposition of crystalline MoS2thinﬁlms: new molybdenum precursor for low-temperature
ﬁlm growth, Adv. Mater. Interfaces 4 (2017) 1700213.
 B. Ballarin, E. Brescacin, G.A. Rizzi, E. Tondello, MoO3thinﬁlms prepared via
MOCVD from a volatile molybdenyl complex, J. Mater. Chem. 5 (1995) 1147e1150.
 M. Nass, M. Schürmann, H. Preut, N. Krause, Crystal structure of cis-dioxo-bis(2,2,6,6-tetramethyl-3,5-heptandionato)-molybdenum(VI), C22H38MoO6,
Z. Kristallogr. New Cryst. Struct. 216 (2001) 461e464.
 Product catalog. Strem Chemicals, Inc. Available at:https://www.strem.com/ catalog/. Accessed April 2018.
 A. Aarik, J. Karlis, H. M€andar, T. Uustare, V. Sammelselg, Inﬂuence of structure development on atomic layer deposition of TiO2thinﬁlms, Appl. Surf. Sci. 181
 W.D. Kim, G.W. Hwang, O.S. Kwon, S.K. Kim, M. Cho, D.S. Jeong, S.W. Lee, M.H. Seo, C.S. Hwang, Y.-S. Min, Y.J. Cho, Growth characteristics of atomic layer deposited TiO2thinﬁlms on Ru and Si electrodes for memory capacitor
applications, J. Electrochem. Soc. 152 (2005). C552.
 S.K. Kim, S. Hoffmann-Eifert, M. Reiners, R. Waser, Relation between enhancement in growth and thickness-dependent crystallization in ALD TiO2
thinﬁlms, J. Electrochem. Soc. 158 (2011). D6.
 Powder Diffraction File (PDF) 5-0508, JCPDS-ICDD, International Center for Diffraction Data, Newtown Square, PA.
 Powder Diffraction File (PDF) 47-1081, JCPDS-ICDD, International Center for Diffraction Data, Newtown Square, PA.
 Powder Diffraction File (PDF) 5-0337, JCPDS-ICDD, International Center for Diffraction Data, Newtown Square, PA.
 Powder Diffraction File (PDF) 13-0142, JCPDS-ICDD, International Center for Diffraction Data, Newtown Square, PA.
 Powder Diffraction File (PDF) 13-0345, JCPDS-ICDD, International Center for Diffraction Data, Newtown Square, PA.
 Powder Diffraction File (PDF) 12-0517, JCPDS-ICDD, International Center for Diffraction Data, Newtown Square, PA.
 Powder Diffraction File (PDF) 5-0339, JCPDS-ICDD, International Center for Diffraction Data, Newtown Square, PA.
 Powder Diffraction File (PDF) 5-0441, JCPDS-ICDD, International Center for Diffraction Data, Newtown Square, PA.
 Powder Diffraction File (PDF) 12-0753, JCPDS-ICDD, International Center for Diffraction Data, Newtown Square, PA.
 M. Birkholz, Thin Film Analysis by X-Ray Scattering, Wiley-VCH, Weinheim, Germany, 2005.
 M. Dieterle, G. Mestl, Raman spectroscopy of molybdenum oxides. Part I. Structural characterization of oxygen defects in MoO3-xby DR UV/VIS, Raman
spectroscopy and X-ray diffraction, Phys. Chem. Chem. Phys. 4 (2002) 812e821.
 T.M. McEvoy, K.J. Stevenson, Spatially resolved imaging of inhomogeneous charge transfer behavior in polymorphous molybdenum oxide. I. Correlation of localized structural, electronic, and chemical properties using conductive probe atomic force microscopy and Raman microprobe spectroscopy, Lang-muir 21 (2005) 3521e3528.
 M. Dieterle, G. Mestl, Raman spectroscopy of molybdenum oxides. Part II. Resonance Raman spectroscopic characterisation of the molybdenum oxides Mo4O11and MoO2, Phys. Chem. Chem. Phys. 4 (2002) 822e826.
 K. Olson, Laser Photodeposition of Molybdenum Oxide Thin Films from Organometallic Precursors (PhD thesis), Iowa State University, 1989.  A. Blume, Synthese und strukturelle untersuchungen von molybd€an-
vana-dium-, und wolfraoxide als referenzverbindungen Fur die heterogene katalyse (PhD thesis), 2004. TU Berlin.
 H. Wu, K. Lian, The development of pseudocapacitive molybdenum oxynitride electrodes for supercapacitors, ECS Trans. 58 (2014) 67e75.
 J. Baltrusaitis, B. Mendoza-Sanchez, V. Fernandez, R. Veenstra, N. Dukstiene, A. Roberts, N. Fairley, Generalized molybdenum oxide surface chemical state XPS determination via informed amorphous sample model, Appl. Surf. Sci. 326 (2015) 151e161.
 A. Szekeres, T. Ivanova, K. Gesheva, Spectroscopic ellipsometry study of CVD molybdenum oxideﬁlms: effect of temperature, J. Solid State Electrochem. 7 (2002) 17e20.
 S. Guimond, D. G€obke, J.M. Sturm, Y. Romanyshyn, H. Kuhlenbeck, M. Cavalleri, H.-J. Freund, Well-ordered molybdenum oxide layers on Au(111): preparation and properties, J. Phys. Chem. C 117 (2013) 8746e8757.  M. Ferroni, V. Guidi, E. Comini, G. Sberveglieri, A. Vomiero, G. Della Mea, G. Martinelli, Selective sublimation processing of a molybdenumetungsten mixed oxide thinﬁlm, J. Vac. Sci. Technol. B 21 (2003) 1442e1448.  Powder Diffraction File (PDF) 32-0671, JCPDS-ICDD, International Center for
Diffraction Data, Newtown Square, PA.
 T. Ressler, R.E. Jentoft, J. Wienold, M.M. Günter, O. Timpe, In situ XAS and XRD studies on the formation of Mo suboxides during reduction of MoO3, J. Phys.
Chem. B 104 (2000) 6360e6370.
 J. Dang, G.H. Zhang, K.C. Chou, Phase transitions and morphology evolutions during hydrogen reduction of MoO3to MoO2, High Temp. Mater. Process. 33